# electro-optic response in germanium halide perovskites · electro-optic response in germanium...

Post on 06-Apr-2018

224 views

Embed Size (px)

TRANSCRIPT

Electro-optic Response in Germanium Halide PerovskitesGrant Walters and Edward H. Sargent*

Department of Electrical and Computer Engineering, University of Toronto, 35 St. George Street, Toronto, Ontario M5S 1A4,Canada

*S Supporting Information

ABSTRACT: Electro-optic materials that can be solution-processed and provide high-crystalline quality are sought for the development of compact, efficient optical modulators.Here we present density functional theory investigations of the linear electro-opticcoefficients of candidate materials cesium and methylammonium germanium halideperovskites. As with their lead halide counterparts, these compounds can be solution-processed, but in contrast, they possess the noncentrosymmetric crystal structures neededto provide a linear electro-optic effect. We find substantial electro-optic responses fromthese compounds; in particular, for the r51 tensor element of CsGeI3, we predict an electro-optic coefficient of 47 pmV1 at the communications wavelength of 1550 nm, surpassingthe strongest coefficient of LiNbO3 at 31 pmV

1. The strong electro-optic responses ofthe germanium compounds are driven by high nonlinear susceptibilities and dynamics ofthe germanium atoms that ultimately arise from the distorted crystal structures. Alongsidethe electro-optic coefficient calculations, we provide the frequency responses for the linearand nonlinear electronic susceptibilities.

The development of efficient, compact electro-opticmodulators for use in intrachip or interchip opticalinterconnects will be further advanced by expanding the set ofelectro-optic materials options. Established inorganic crystals,chiefly LiNbO3 and BaTiO3, are fabricated using processingtechniques, such as Czochralski crystal growth or epitaxialMOCVD, that limit compatibility with standard siliconphotonics. Organic materials are deposited via inexpensiveand simple solution-processing methods and have performedimpressively when incorporated within pioneering modulatorarchitectures such as silicon slot-waveguide interferometers.1,2

Unfortunately, the electrostatic poling of the organic moleculesthat is needed to orient and maintain orientation of themolecules has limited their breadth of application to date.These limitations motivate the search for new solution-

processed materials that exhibit strong, built-in, electro-opticactivity.Recently, metal halide perovskites have risen as solution-

processed materials with impressive electrical and opticalproperties. These materials, possessing the chemical formulaABX3 (where A is a cation, B is a metal cation, and X is a halideanion), have demonstrated impressive performance in a broadrange of optoelectronic devices.36 Elements of the success ofmetal halide perovskites can be traced to their flexibility incomposition and morphology. The optical, electrical, andstructural properties can be finely tuned through differentcombinations of cations and anions.7,8 Various solution-processing methods can be used to grow different forms ofperovskites: quantum-confined nanostructures,911 polycrystal-line thin films,12 and macroscopic single crystals.13,14

The nonlinear optical properties are much less explored thantheir behavior as light-absorbing and light-emitting materials.

The widely researched metal halide perovskites, particularly thelead-based ones, are structurally globally centrosymmetric andtherefore are incapable of some nonlinear optical processes,including the linear electro-optic (LEO) effect.The germanium halide perovskites are a class of non-

centrosymmetric compounds. As in the case of lead,germanium is a group IV element that is capable of carryinga 2+ valence state. However, its higher position within theperiodic column lends the 4s electron pair greater stereo-chemical activity when compared to the lead analogue.15 Thisactivity distorts the perovskite unit cell, causing it to lose itsinversion symmetry. The germanium halide perovskites aredrawing increased interest as lead-free alternatives for photo-voltaic application1619 and have also previously been reportedto exhibit impressive second-harmonic generation (SHG),2024

a phenomenon intimately linked with LEO. Motivated by thisfact, combined with their transparency over the infraredcommunications wavelengths20,25,26 and evidence for growthof crystals from solution,20,22,23,25,27,28 we investigate herein theelectro-optic and nonlinear optical behavior for germaniumhalide perovskites using density functional theory calculations.We focus our study on cesium germanium halides (CsGeX3;

X = I, Br, Cl) and methylammonium germanium iodide(MAGeI3). We provide predictions for the LEO coefficientsand, by examining the factors contributing to the electro-opticbehavior and the trends associated with the halide anions and Acations, provide mechanistic insights into the LEO responses.We complement these predictions with calculations of the

Received: December 19, 2017Accepted: February 9, 2018Published: February 9, 2018

Letter

pubs.acs.org/JPCLCite This: J. Phys. Chem. Lett. 2018, 9, 10181027

XXXX American Chemical Society 1018 DOI: 10.1021/acs.jpclett.7b03353J. Phys. Chem. Lett. 2018, 9, 10181027

pubs.acs.org/JPCLhttp://pubs.acs.org/action/showCitFormats?doi=10.1021/acs.jpclett.7b03353http://dx.doi.org/10.1021/acs.jpclett.7b03353

linear and nonlinear susceptibilities and their frequencyresponses.As in other metal halide perovskites, germanium-based

perovskites assemble as an inorganic network of metal halideoctahedra surrounding their A-site cations, such as methyl-ammonium or cesium cations. However, in contrast with mostother perovskites, those based on germanium have a distortedunit cell: they reside in the noncentrosymmetric trigonal R3mspace group.20,22,23,27,29 The rhombohedral representation ofthe crystal structure is provided in Figure 1ac. The angularlattice parameter of the unit cell deviates only slightly from 90.The A cations occupy the corners, the halide species occupypositions near the face centers, and the germanium atoms

occupy positions offset along the [111] direction from the bodycenters. For compounds with the polar molecular methyl-ammonium, which possesses C3v symmetry, the molecules CN axis aligns along the [111] direction.20 The atomic offsetsyield two distinct GeX bonds. Notably, the central offset ofthe germanium cations is reminiscent of that for titanium atomsin the electro-optic material BaTiO3.Calculations of the structural parameters (Figure 1df and

Table S1) agree with the experimental findings for synthesizedmicrocrystals.20,22,23,27,29 Unsurprisingly, the cesium com-pounds show that as the size of the halide anion increases,the unit cell expands. The unit cells angular deviation grows asthe cell expands. MAGeI3 has a similar lattice constant as itscesium counterpart, but it exhibits a much greater angulardistortion. The germanium atoms offset from the body-centerincreases as the halide size increases. Accompanying this is achange in the offset of the halide species from the face-centersthat lessens the discrepancy between the two lengths of GeXbonds.Electro-optic materials, to be of use in optical communica-

tions systems, are required to be optically transparent across theinfrared communications bands. As in the case of most metalhalide perovskites, the electronic bandgaps of the germaniumcompounds decrease as the halide size increases and lie withinthe visible spectrum. Substitution of cesium cations withmethylammonium leads to widening of the bandgap, which haspreviously been attributed to further stereochemical activitionof the germanium 4s2 lone pair.20

We calculated the bandgaps at the levels of the LDA, GGA,and HSE06 approximations (Table 1). We further calculated

the real and imaginary components of the dielectric function,(), at optical frequencies (atomic positions are clamped) atthe LDA level using scissors corrections set to theexperimentally reported bandgaps; the response curves areprovided in Figure 2. The use of scissors corrections isnecessary due to the problem of bandgap underestimation inDFT and the consequent overestimation of the dielectricproperties.21,30,31 The corrections act as rigid shifts to theconduction bands in order to curtail bandgap estimation andhave been widely used in calculations of linear and nonlinearoptical properties of many materials.21,3046 As empiricaladjustments, these corrections introduce a degree ofuncertainty to the calculations; however, as we show below,these corrections are validated by the strong agreementbetween the scissors-corrected and experimental SHG charac-teristics.The germanium materials possess uniaxial birefringence and

refractive indices that scale with bandgap. Along with thedielectric functions, we have plotted the electronic bandstructures in Figure 3. All of the germanium compoundsexhibit a direct bandgap at the Brillouin zone Z point; therhombohedral nature of these crystals changes the gap from theR point of cubic perovskite phases.47 The first few optical

Figure 1. Structural representations of the rhombohedral lattice forgermanium halide perovskites: (a) standard orientation, (b) [100]view, (c) [111] view showing hexagonal symmetry. Red, black, andwhite spheres are Ge2+ cations, A+ cations, and X halide anions,respectively. Calculated structural parameters: (d) lattice constant, (e)lattice angular parameter, (f) XYZ coordinate of the near-body-centerGe atoms. Experimental results are taken from refs 20 and 22.

Table 1. Calculated Bandgap Values (eV)

compound LDA GGA HSE06 exp.

CsGeCl3 2.01 2.21 2.22 3.43a

CsGeBr3 1.26 1.53 1.66 2.38a

CsGeI3 0.66 1.19 1.41 1.6b

MAGeI3 0.37 1.52 1.84 1.9b

aReference 22. bReference 20.

The Journal of Physical Chemistry Letters Letter

DOI: 10.1021/acs.jpclett.7b03353J. Phys. Chem. Lett. 2018, 9, 10181027

1019

http://pubs.acs.org/doi/suppl/10.1021/acs.jpclett.7b03353/suppl_file/jz7b03353_si_001.pdfhttp://dx.doi.org/10.1021/acs.jpclett.7b03353

transitions can be connected with spectral features in theimaginary dielectric functions.The LEO effect is the special case of second-order nonlinear

optical processes where one of the interacting electric fields islow-frequency while the other remains at optical frequencies.Changes to the optical dielectric constants can be induced bythe low-frequency electric fields and are related through LEOcoefficients. The LEO effect on the optical dielectric constant isdefined by the following relation

=

=

r E( )ij ij1

1

3

(1)

where rij are the LEO coefficients and E are electric fieldcomponents (Greek indices correspond to static directionalfields, and Latin indices correspond to optical directionalfields). The LEO coefficients are the central figures of merit forelectro-optic materials; a large LEO coefficient is key forefficient electro-optic modulation. The LEO coefficients of amaterial can be calculated with density functional perturbationtheory (DFPT), as formulated by Veithen et al.30 Bydetermining the energetic changes induced by atomic displace-ments and homogeneous electric fields using DFT calculations,the electro-optic coefficients can be found.The LEO coefficients at telecommunications bandwidths

(i.e., field frequencies above 100 MHz) are formed from twocontributions: an electronic, rij

el , and an ionic, rijion, response.30

Within the BornOppenheimer approximation, these twoquantities sum to form the total LEO coefficient. The electroniccontribution is due to field interactions with the valenceelectrons while considering the ions as clamped. This term isrelated to the LEO second-order susceptibility, ijk

(2)(;,0),via

= =

rn n

8( ; , 0)ij

i jijk k

el2 2

(2)

(2)

where n are refractive indices.30 We note that the DFTcalculations of this term neglect the dispersion of the second-

order susceptibility, and therefore, the term typically presents alower bound. The ionic contribution accounts for the relaxationof the atomic positions due to the electric field and thecorresponding dielectric changes. This term is given by a sumover the transverse optic phonon modes (indexed by m)

=

r

n n

p4ij

i j m

ijm

m

m

ion

02 2

,2

(3)

where 0 is the unit cell volume, ijm are the Ramansusceptibility components for the modes, pm, are the modepolarities, and m are the mode frequencies.

30 The Ramansusceptibilities are found from a sum over the products of thechanges in susceptibility resulting from atomic displacements,ij

(1)/,, and the modal atomic eigendisplacements, um(),for all atoms (indexed by )30

=

u ( )ij

m ij0

,

(1)

,m

(4)

The mode polarities are given by a similar sum over theproducts of the Born effective charges, Z,* , and the modalatomic eigendisplacements30

= *

p Z u ( )m,,

, m(5)

Two quantities central to the DFPT LEO calculations are thelinear and second-order nonlinear susceptibilities. Table 2 givesthe calculated optical (, atomic positions clamped) and static(0, atomic positions unclamped) zero-frequency dielectricconstants at the LDA level with and without scissorscorrections. The dielectric constants reflect the sameconclusions drawn from the calculated dielectric functionspreviously shown. As expected, the scissors corrections alsoreduce the dielectric constants and therefore will play a role inthe determination of the LEO coefficients. Table 3 provides theLEO nonlinear susceptibilities, given as dij = ij

(2)/2 usingcontracted indices, with and without scissors corrections. Again,

Figure 2. Calculated dielectric functions for germanium halide perovskites. (a) Real ordinary components. (b) Real extraordinary components. (c)Imaginary ordinary components. (d) Imaginary extraordinary components. Lettering on the curves for CsGeI3 is used to connect with the electronicband dispersion plot. Calculations have been done with LDA exchangecorrelation functionals and have been scissors-corrected.

The Journal of Physical Chemistry Letters Letter

DOI: 10.1021/acs.jpclett.7b03353J. Phys. Chem. Lett. 2018, 9, 10181027

1020

http://dx.doi.org/10.1021/acs.jpclett.7b03353

the bandgap correction generates a considerable difference.Akin to the linear susceptibilities, the nonlinear susceptibilitiesincrease as the size of the halide anion increases. Substitution ofcesium with methylammonium leads to a decrease in thenonlinear susceptibilities. Thus, inspection of all of thecompounds shows simply the expected scaling of the nonlinear

susceptibility with bandgap.48 Interestingly, the greatest non-linear susceptibility component for CsGeCl3 and CsGeBr3 isthe d33, while for CsGeI3 and MAGeI3 it is the d13.These calculations of the electronic susceptibilities, along

with the ionic terms calculated by atomic perturbationcalculations, were then used to obtain the LEO coefficients.The space group for the germanium compounds yields eightnonzero tensor components, of which four are unique (FigureS1); these happen to be the same components possessed byLiNbO3. The coefficients for each germanium compound areprovided in Table 4. The contributions from each set of ionictransverse optical (TO) phonon modes and from the electronicresponses are listed at the LDA level. We have furthercalculated the final coefficients at two different levels of scissorscorrections. The first, SCI1, uses the scissors-correcteddielectric constants. The second, SCI2, uses scissors-correctedvalues for both the dielectric constants and the nonlinearsusceptibilities. We note that this means that we have only usedscissors corrections for quantities calculated from electric fieldperturbations. The differences between the quantities obtainedwith the different levels of correction illustrate the uncertaintyof the calculations; however, considering the available reportsof the experimental effective SHG nonlinear susceptibilities forthese materials at optical frequencies,20,22,23 we believe that themore modest values of the LEO susceptibilities obtained withthe scissors corrections are more accurate, and therefore, SCI2stands as the most accurate prediction of the LEO response.We provide a plot to illustrate trends in the electronic and ionicresponses with this level of correction in Figure 4. All of thegermanium compounds exhibit significant LEO responses;CsGeI3 possesses a component (r51 = 37.64 pmV

1) that evenexceeds the strongest component for LiNbO3 (experimental r33= 30.8 pmV1 at 633 nm;49 SCI2 calculation 27.28 pmV1; seeTable S2). This is particularly remarkable considering thatthese calculated values exclude any frequency dependence andtherefore represent a lower bound. For the cesium compounds,the LEO response tends to increase as the halide size increases;

Figure 3. Calculated electronic band diagrams for germanium halideperovskites: (a) CsGeI3, (b) CsGeBr3, (c) CsGeCl3, and (d) MAGeI3.The first few optical transitions have been indicated for CsGeI3.Scissors corrections have been applied, and LDA functionals wereused.

Table 2. Optical and Static Linear Dielectric PropertiesObtained from 2n + 1 Theorem DFPT Calculations

compound 11,220 33

0 11,22 33

CsGeCl3 LDA 9.87 9.05 3.85 3.69SCI 9.32 8.54 3.30 3.18

CsGeBr3 LDA 12.00 11.30 5.07 4.96SCI 11.28 10.56 4.34 4.22

CsGeI3 LDA 14.97 14.87 7.48 7.69SCI 13.53 13.13 6.04 5.95

MAGeI3 LDA 15.26 7.54 5.36 5.42SCI 14.53 6.73 4.63 4.61

Table 3. LEO Nonlinear Susceptibilities (pmV1) Obtainedfrom 2n + 1 Theorem DFPT Calculations

compound d11 d13 d33

CsGeCl3 LDA 1.0 4.6 9.5SCI 0.1 2.0 4.8

CsGeBr3 LDA 9.9 16.7 21.6SCI 4.1 8.5 12.9

CsGeI3 LDA 104.3 173.4 32.9SCI 33.9 50.6 12.1

MAGeI3 LDA 32.0 44.9 8.9SCI 13.6 20.1 10.3

The Journal of Physical Chemistry Letters Letter

DOI: 10.1021/acs.jpclett.7b03353J. Phys. Chem. Lett. 2018, 9, 10181027

1021

http://pubs.acs.org/doi/suppl/10.1021/acs.jpclett.7b03353/suppl_file/jz7b03353_si_001.pdfhttp://pubs.acs.org/doi/suppl/10.1021/acs.jpclett.7b03353/suppl_file/jz7b03353_si_001.pdfhttp://pubs.acs.org/doi/suppl/10.1021/acs.jpclett.7b03353/suppl_file/jz7b03353_si_001.pdfhttp://dx.doi.org/10.1021/acs.jpclett.7b03353

this is primarily driven by the corresponding increases to theelectronic contribution. Smaller differences are observed in theionic contributions. These differences are most noticeablebetween CsGeI3 and MAGeI3, where the methylammoniumcompound has a considerably smaller ionic contribution andtherefore a much weaker LEO response.Further insight into the ionic contributions can be gained by

inspecting the modal parts and their characteristics. First weconsider the Born effective charges (Table S3). The effectivecharges are defined as the changes in polarization that resultfrom atomic displacements and are factors that control theCoulombic interactions between nuclei.50,51 They are indicativeof the influence of dynamical changes to orbital hybridizationcaused by atomic displacements.50,51 For the germanium

perovskites, as the size of the halide anion increases, theeffective charges deviate more from their nominal charges (A+,Ge2+, X), especially for the Ge and X atoms, indicating thatthe bonds become more covalent and sensitive to atomicdisplacements. The vibrational modes involving more covalentbonds would then have a greater electro-optic response.MAGeI3 has bonds with more ionic character than all of thecesium compounds, and the methylammonium cation is almostcompletely ionized.Next we consider the characteristics of each mode. The

vibrational frequencies of the modes are provided in Table S4,and the modal atomic eigendisplacements are provided inTables S5S8. First, we note that the modal frequencies followan expected Hookean-type relation to the mass of the halide

Table 4. Clamped Linear EO Coefficients (pmV1) Obtained from 2n + 1 Theorem DFPT Calculationsa

E modes A1 modes

compound contribution r11 r51 r13 r33

CsGeCl3 TO1 46 0.75 0.42 43 0.45 0.64TO2 76 0.08 0.20 66 b bTO3 121 0.20 0.18 148 0.95 1.08TO4 213 6.83 10.53 253 5.06 5.62ionic 5.96 9.73 3.66 5.18electronic 0.27 1.29 1.24 2.80total 6.23 11.02 4.90 7.98total (SCI1) 8.46 14.90 6.65 10.75total (SCI2) 8.14 13.92 5.71 8.88

CsGeBr3 TO1 43 0.21 0.78 35 0.10 0.79TO2 53 0.04 0.10 49 b bTO3 79 0.22 0.36 93 0.17 0.25TO4 145 11.47 18.07 174 7.72 8.55ionic 11.42 18.39 7.45 9.09electronic 1.54 2.65 2.60 3.43total 12.96 21.04 10.04 12.52total (SCI1) 17.68 28.89 13.70 17.29total (SCI2) 16.45 27.12 11.98 15.45

CsGeI3 TO1 35 0.62 0.88 27 0.28 0.16TO2 42 0.00 0.00 39 b bTO3 60 0.61 0.80 70 0.67 0.50TO4 126 12.43 19.94 147 6.04 5.67ionic 12.44 20.02 6.44 6.01electronic 7.45 12.05 12.39 2.23total 19.89 32.07 18.83 3.79total (SCI1) 30.48 51.30 28.85 6.32total (SCI2) 22.77 37.64 15.40 11.40

MAGeI3 TO1 18 3.00 0.16 15 b bTO2 45 0.17 0.26 73 2.54 2.25TO3 57 0.86 0.98 121 1.60 1.26TO4 92 0.19 1.18 124 b bTO5 144 6.64 10.99 163 3.13 3.16TO6 869 0.02 0.02 335 b bTO7 1215 0.00 0.00 1004 0.00 0.00TO8 1431 0.01 0.01 1394 0.00 0.00TO9 1561 0.00 0.00 1445 0.04 0.04TO10 2762 0.01 0.02 2792 0.01 0.05TO11 2922 0.00 0.00 2857 0.01 0.00ionic 2.73 8.91 4.03 4.24electronic 4.45 6.18 6.24 1.21total 7.17 15.09 10.28 5.45total (SCI1) 9.62 20.53 13.78 7.52total (SCI2) 6.19 15.89 9.16 7.78

aMode phonon frequencies of ionic contributions are expressed in cm1. bNot Raman-active.

The Journal of Physical Chemistry Letters Letter

DOI: 10.1021/acs.jpclett.7b03353J. Phys. Chem. Lett. 2018, 9, 10181027

1022

http://pubs.acs.org/doi/suppl/10.1021/acs.jpclett.7b03353/suppl_file/jz7b03353_si_001.pdfhttp://pubs.acs.org/doi/suppl/10.1021/acs.jpclett.7b03353/suppl_file/jz7b03353_si_001.pdfhttp://pubs.acs.org/doi/suppl/10.1021/acs.jpclett.7b03353/suppl_file/jz7b03353_si_001.pdfhttp://dx.doi.org/10.1021/acs.jpclett.7b03353

anions, so that the iodide compounds benefit the most from theinverse relation of the electro-optic response to the modalfrequency squared. We see that the modes involving thecovalent germanium halide bonds and displacements of thegermanium atoms possess the greatest electro-optic activity.The displacement of these atoms, having large effective charges,leads to strong modal oscillator strengths (Table S9) andRaman susceptibilities (Tables S10 and S11). These trendsthen propagate to those observed for the electro-optic activity.Looking at the cesium compounds, the first set of transverseoptical modes (modes 46, TO1) involves movements of thewhole germanium halide octahedra and therefore exhibits weakLEO responses. The second set of transverse optical modes(modes 79, TO2) consists of an inactive symmetric mode anda doubly degenerate mode involving small germaniumdisplacements and complex motions of the halide anions; thethird set of transverse optical modes (modes 1012, TO3)involves similar motions as the formers doubly degeneratemode. Altogether, the TO2 and TO3 modes have weak LEOresponses. The fourth set of transverse optical modes (modes1315, TO4) involves large displacements of the germaniumatoms and therefore dominates the ionic LEO response.MAGeI3 has similar vibrational modes as CsGeI3 but also hashigh-frequency modes relating to the internal degrees of

freedom of the methylammonium cations. These additionalmodes have exceptionally small LEO responses. Furthermore,the strong ionic character of this compound softens the LEOresponse of the modes involving germanium and halogenmovements.As a complement to our calculations of the LEO coefficients,

we have calculated the frequency responses of the SHG andLEO second-order electronic susceptibilities (ijk

(2)(2;,)and ijk

(2)(;,0) respectively). The below-bandgap absoluteresponse curves are provided in Figure 5ad for the LEO andSHG tensor components of the strongest LEO coefficients andfor the effective SHG susceptibilities at the scissors-correctedLDA level. The full frequency responses of the strongest SHGsusceptibility tensor components are provided in Figure 5e.The effective SHG susceptibilities rely on all of the tensorcomponents and correspond to the values measurable withpowder-SHG experiments. Prior reports of the effective SHGsusceptibility at particular wavelengths agree well with ourfrequency response calculations: MAGeI3 eff

(2)(2;,) = 161pmV1 at 0.7 eV,20 CsGeI3 eff(2)(2;,) = 125 pmV1 at0.7 eV,20 CsGeBr3 eff(2)(2;,) 18 pmV1 at 0.98 eV,

22

and CsGeCl3 eff(2)(2;,) 2 pmV1 at 0.98 eV.22 This

agreement also justifies the necessity of the scissors corrections(see Figure S2). The LEO susceptibilities display frequencydependence that translates to dependence in the electroniccontributions of the LEO coefficients (Figure 5f). Accountingfor this and the linear susceptibility dispersion, the r51 LEOcoefficient of CsGeI3 will then increase to 47 pmV

1 at thetelecommunications band of 1550 nm.In summary, we have determined that the germanium halide

perovskites exhibit significant electro-optic responses that forsome compounds are on par with or even exceed that of thearchetypal electro-optic material LiNbO3. The intrinsicallydistorted nature of the structures leads to nonlinear electronicsusceptibilities and dynamics of the germanium and halogenatoms that drive the electro-optic activity. The nonlinearsusceptibilities and electro-optic responses are strongest for theiodide compounds and scale with bandgap. The ioniccontributions to the electro-optic characteristics are strongly

Figure 4. Calculated ionic and electronic LEO responses with scissors-corrected linear and nonlinear susceptibilities (SCI2).

Figure 5. Calculated frequency response of the electronic nonlinear susceptibility. Below-bandgap responses for the effective SHG susceptibility andthe SHG and LEO susceptibilities for the strongest LEO tensor components for (a) CsGeI3, (b) CsGeBr3, (c) CsGeCl3, and (d) MAGeI3. (e) Fullfrequency responses of the effective SHG susceptibility. (f) Normalized frequency response of the strongest electronic LEO terms for eachgermanium compound. Calculations were done at the level of the LDA and have been scissors-corrected.

The Journal of Physical Chemistry Letters Letter

DOI: 10.1021/acs.jpclett.7b03353J. Phys. Chem. Lett. 2018, 9, 10181027

1023

http://pubs.acs.org/doi/suppl/10.1021/acs.jpclett.7b03353/suppl_file/jz7b03353_si_001.pdfhttp://pubs.acs.org/doi/suppl/10.1021/acs.jpclett.7b03353/suppl_file/jz7b03353_si_001.pdfhttp://pubs.acs.org/doi/suppl/10.1021/acs.jpclett.7b03353/suppl_file/jz7b03353_si_001.pdfhttp://dx.doi.org/10.1021/acs.jpclett.7b03353

influenced by the covalency of the germanium halide bonds andthe vibrational properties of the germanium and halogen atoms.Substitution of cesium with methylammonium is detrimental tothe ionic response as the bonds become more ionic and theinternal vibrations of methylammonium do not contribute. Thestrong electro-optic performance of the germanium halideperovskites, compounded by their solution-processability,makes them attractive candidates for use in optical modulators.The realization of germanium halide perovskite optical

modulators requires surmounting of a number of experimentalchallenges. Crystallization techniques must be developed forthese materials that produce high-quality macroscopic singlecrystals. Bulk characterization and implementation in a practicalmodulator will require approximately an order of magnitudeincrease in crystal dimensions over the crystals produced fromknown techniques, which possess dimensions less than 100m.20,28 As well, the crystals must also be of high optical qualityin order to prevent any influence of internal or surfacescattering on the optical characterization. Recent advances incrystallizing the broader spectrum of metal halide perovskitessuggest promising avenues.14,5255 Techniques must also bedeveloped for the deposition or growth of the crystals on amodulator platform. The crystals will need to be preciselyoriented with the device architecture and have excellent highoptical quality in order to maximize the device efficiency. Again,recent reports on lead halide perovskites are encouraging in thisregard.5660 The present study may help to motivate futureendeavors to advance the crystallization and depositiontechniques of the germanium halide perovskites with the aimof developing optical modulators.

COMPUTATIONAL METHODSCalculations of the nonlinear response functions were donewithin density functional perturbation theory, employing the 2n+ 1 theorem, as developed by Veithen et al.30 and implementedin the ABINIT software package.6166 The package cancurrently only implement nonlinear response function calcu-lations in the Local Density Approximation (LDA) with norm-conserving pseudopotentials. These calculations include thestatic and optical dielectric constants, the nonlinear opticalcoefficients, the electro-optic coefficients, and the quantitiesrequired in their derivation. Self-consistent calculations weredone in the LDA with the exchangecorrelation functionalPerdewWang 92 parametrization.67 Norm-conserving pseu-dopotentials generated using the TroullierMartins method68were used. Calculations were done with the experimental latticeconstants and with atomic positions relaxed such that maximalforces were less than 106 Habohr1. Where indicated, ascissors correction has been applied for all calculations toaccount for the LDA underestimation of the bandgap andconsequent overestimation of the dielectric properties. Thescissors corrections have been included at two different levels:SCI1, which includes scissors-corrected dielectric constants,and, SCI2, which includes scissors-corrected dielectric con-stants and nonlinear susceptibilities. The Brillouin zone wassampled using a MonkhorstPack 18 18 18 grid of specialk-points, and wave functions were expanded in plane-waves upto a kinetic energy cutoff of 60 Ha. These parameters werefound to be necessary for convergence of the electro-opticcoefficients. The calculations of the electro-optic coefficientswere benchmarked against calculations for LiNbO3, which areprovided in Table S2. These results agree well with prior DFTcalculations30 and with experimental findings.49

The frequency-dependent optical responses were calculatedwith the ABINIT6166 package Optic following work byHughes and Sipe,35 which uses the independent particleapproximation. These calculations include the dielectricfunction (), the second-harmonic generation (SHG)susceptibility (2)(2;,), and the LEO susceptibility(2)(0;,). The LEO susceptibility is calculated in theclamped-lattice approximation, which corresponds to theintermediate frequency regime where lattice vibrations arefrozen out and electronic dispersion can be neglected. Self-consistent calculations were done in the LDA with theexchangecorrelation functional PerdewWang 92 parametri-zation.67 Norm-conserving pseudopotentials generated usingthe TroullierMartins method68 were used. Calculations weredone with the experimental lattice constants and with atomicpositions relaxed such that maximal forces were less than 106

Habohr1. A scissors correction has been applied for allcalculations to account for the LDA underestimation of thebandgap. The Brillouin zone was sampled using a MonkhorstPack 26 26 26 grid of special k-points, wave functions wereexpanded in plane-waves up to a kinetic energy cutoff of 20 Ha,and the number of bands included was 36 for the inorganiccompounds and 40 for the methylammonium compound.These parameters were found to be necessary for convergenceof the nonlinear susceptibilities. The effective nonlinearcoefficients were calculated based on relations provided byKurtz and Perry.69

Band structure calculations were conducted through ABINITusing the same parameters as in the preceding paragraph. TheBrillouin zone was sampled following a k-path for rhombohe-dral structures as described in ref 70.Hybrid DFT calculations of the bandgaps were done with the

Quantum Espresso71 implementation package. Norm-conserv-ing pseudopotentials with PerdewBurkeErnzerhof72 ex-changecorrelations generated with the MartinsTroulliermethod68 were combined with HSE06 hybrid functionals,73,74

and 0.25 exchange fractions and 0.106 screening parameterswere used. Lattice constants and atomic positions weresimultaneously relaxed, such that forces were less than 2 106 Habohr1 and pressures were less than 0.5 kbar, prior tohybrid calculations. An 8 8 8 MonkhorstPack k-pointgrid and 2 2 2 q-point grid were used with an energy cutoffof 30 Ha for the hybrid calculations.Atomic illustrations were produced with the visualization

software VESTA.75

ASSOCIATED CONTENT*S Supporting InformationThe Supporting Information is available free of charge on theACS Publications website at DOI: 10.1021/acs.jpclett.7b03353.

Imaginary components of the SHG susceptibility,structural parameters following relaxation, lithiumniobate benchmark, Born effective charges, atomiceigendisplacements, phonon frequencies, mode oscillatorstrengths, mode effective charges, and modal Ramansusceptibilities (PDF)

AUTHOR INFORMATIONCorresponding Author*E-mail: [email protected] Walters: 0000-0002-9005-2335

The Journal of Physical Chemistry Letters Letter

DOI: 10.1021/acs.jpclett.7b03353J. Phys. Chem. Lett. 2018, 9, 10181027

1024

http://pubs.acs.org/doi/suppl/10.1021/acs.jpclett.7b03353/suppl_file/jz7b03353_si_001.pdfhttp://pubs.acs.orghttp://pubs.acs.org/doi/abs/10.1021/acs.jpclett.7b03353http://pubs.acs.org/doi/suppl/10.1021/acs.jpclett.7b03353/suppl_file/jz7b03353_si_001.pdfmailto:[email protected]://orcid.org/0000-0002-9005-2335http://dx.doi.org/10.1021/acs.jpclett.7b03353

NotesThe authors declare no competing financial interest.

ACKNOWLEDGMENTSThe work presented in this publication was supported byfunding from an award (KUS-11-009-21) from the KingAbdullah University of Science and Technology, the OntarioResearch Fund, the Ontario Research Fund ResearchExcellence Program, and the Natural Sciences and EngineeringResearch Council (NSERC) of Canada. Computations wereperformed on the General Purpose Cluster supercomputer atthe SciNet HPC Consortium. SciNet is funded by the CanadaFoundation for Innovation under the auspices of ComputeCanada; the Government of Ontario; Ontario Research Fund -Research Excellence; and the University of Toronto. Theauthors thank O. Voznyy and A. Jain for useful discussions.

REFERENCES(1) Koeber, S.; Palmer, R.; Lauermann, M.; Heni, W.; Elder, D. L.;Korn, D.; Woessner, M.; Alloatti, L.; Koenig, S.; Schindler, P. C.; et al.Femtojoule Electro-Optic Modulation Using a SiliconOrganicHybrid Device. Light: Sci. Appl. 2015, 4, e255.(2) Alloatti, L.; Palmer, R.; Diebold, S.; Pahl, K. P.; Chen, B.; Dinu,R.; Fournier, M.; Fedeli, J.-M.; Zwick, T.; Freude, W.; et al. 100 GHzSiliconorganic Hybrid Modulator. Light: Sci. Appl. 2014, 3, e173.(3) Yang, W. S.; Park, B.-W.; Jung, E. H.; Jeon, N. J.; Kim, Y. C.; Lee,D. U.; Shin, S. S.; Seo, J.; Kim, E. K.; Noh, J. H.; et al. IodideManagement in Formamidinium-Lead-Halidebased PerovskiteLayers for Efficient Solar Cells. Science 2017, 356 (6345), 13761379.(4) Jia, Y.; Kerner, R. A.; Grede, A. J.; Rand, B. P.; Giebink, N. C.Continuous-Wave Lasing in an Organicinorganic Lead HalidePerovskite Semiconductor. Nat. Photonics 2017, 11 (12), 784788.(5) Xiao, Z.; Kerner, R. A.; Zhao, L.; Tran, N. L.; Lee, K. M.; Koh, T.-W.; Scholes, G. D.; Rand, B. P. Efficient Perovskite Light-EmittingDiodes Featuring Nanometre-Sized Crystallites. Nat. Photonics 2017,11 (2), 108115.(6) Yuan, M.; Quan, L. N.; Comin, R.; Walters, G.; Sabatini, R.;Voznyy, O.; Hoogland, S.; Zhao, Y.; Beauregard, E. M.; Kanjanaboos,P.; et al. Perovskite Energy Funnels for Efficient Light-EmittingDiodes. Nat. Nanotechnol. 2016, 11 (10), 872877.(7) Liao, Y.; Liu, H.; Zhou, W.; Yang, D.; Shang, Y.; Shi, Z.; Li, B.;Jiang, X.; Zhang, L.; Quan, L. N.; et al. Highly Oriented Low-Dimensional Tin Halide Perovskites with Enhanced Stability andPhotovoltaic Performance. J. Am. Chem. Soc. 2017, 139 (19), 66936699.(8) Li, W.; Wang, Z.; Deschler, F.; Gao, S.; Friend, R. H.; Cheetham,A. K. Chemically Diverse and Multifunctional Hybrid Organicinorganic Perovskites. Nat. Rev. Mater. 2017, 2 (3), 16099.(9) Protesescu, L.; Yakunin, S.; Bodnarchuk, M. I.; Krieg, F.; Caputo,R.; Hendon, C. H.; Yang, R. X.; Walsh, A.; Kovalenko, M. V.Nanocrystals of Cesium Lead Halide Perovskites (CsPbX3, X = Cl, Br,and I): Novel Optoelectronic Materials Showing Bright Emission withWide Color Gamut. Nano Lett. 2015, 15 (6), 36923696.(10) Kovalenko, M. V.; Protesescu, L.; Bodnarchuk, M. I. Propertiesand Potential Optoelectronic Applications of Lead Halide PerovskiteNanocrystals. Science 2017, 358 (6364), 745750.(11) Weidman, M. C.; Seitz, M.; Stranks, S. D.; Tisdale, W. A. HighlyTunable Colloidal Perovskite Nanoplatelets through Variable Cation,Metal, and Halide Composition. ACS Nano 2016, 10 (8), 78307839.(12) Jeon, N. J.; Noh, J. H.; Kim, Y. C.; Yang, W. S.; Ryu, S.; Seok, S.I. Solvent Engineering for High-Performance InorganicorganicHybrid Perovskite Solar Cells. Nat. Mater. 2014, 13 (9), 897903.(13) Shi, D.; Adinolfi, V.; Comin, R.; Yuan, M.; Alarousu, E.; Buin,A.; Chen, Y.; Hoogland, S.; Rothenberger, A.; Katsiev, K.; et al. LowTrap-State Density and Long Carrier Diffusion in OrganoleadTrihalide Perovskite Single Crystals. Science 2015, 347 (6221), 519522.

(14) Liu, Y.; Yang, Z.; Cui, D.; Ren, X.; Sun, J.; Liu, X.; Zhang, J.;Wei, Q.; Fan, H.; Yu, F.; et al. Two-Inch-Sized PerovskiteCH3NH3PbX3 (X = Cl, Br, I) Crystals: Growth and Characterization.Adv. Mater. 2015, 27 (35), 51765183.(15) Galy, J.; Meunier, G.; et al. Stereochimie Des ElementsComportant Des Paires Non Liess: Ge (II), As (III), Se (IV), Br (V),Sn (II), Sb (III), Te (IV), I (V), Xe (VI), Tl (I), Pb (II), et Bi (III)(Oxydes, Fluorures et Oxyfluorures). J. Solid State Chem. 1975, 13,142159.(16) Krishnamoorthy, T.; Ding, H.; Yan, C.; Leong, W. L.; Baikie, T.;Zhang, Z.; Sherburne, M.; Li, S.; Asta, M.; Mathews, N.; et al. Lead-Free Germanium Iodide Perovskite Materials for PhotovoltaicApplications. J. Mater. Chem. A 2015, 3 (47), 2382923832.(17) Sun, P.-P.; Li, Q.-S.; Yang, L.-N.; Li, Z.-S. Theoretical Insightsinto a Potential Lead-Free Hybrid Perovskite: Substituting Pb 2+ withGe 2+. Nanoscale 2016, 8 (3), 15031512.(18) Zhao, Y.-Q.; Liu, B.; Yu, Z.-L.; Cao, D.; Cai, M.-Q. TuningCharge Carrier Types, Superior Mobility and Absorption in Lead-FreePerovskite CH3NH3GeI3: Theoretical Study. Electrochim. Acta 2017,247, 891898.(19) Roknuzzaman, M.; Ostrikov, K.; Wang, H.; Du, A.;Tesfamichael, T. Towards Lead-Free Perovskite Photovoltaics andOptoelectronics by Ab-Initio Simulations. Sci. Rep. 2017, 7, 14025.(20) Stoumpos, C. C.; Frazer, L.; Clark, D. J.; Kim, Y. S.; Rhim, S. H.;Freeman, A. J.; Ketterson, J. B.; Jang, J. I.; Kanatzidis, M. G. HybridGermanium Iodide Perovskite Semiconductors: Active Lone Pairs,Structural Distortions, Direct and Indirect Energy Gaps, and StrongNonlinear Optical Properties. J. Am. Chem. Soc. 2015, 137 (21), 68046819.(21) Huang, C. B.; Wang, Z. Y.; Wu, H. X.; Ni, Y. B.; Xiao, R. C.; Qi,M. Ab Initio Study of the Linear and Nonlinear Optical Properties ofHexagonal CdSe. Comput. Condens. Matter 2015, 3, 4145.(22) Lin, Z.-G.; Tang, L.-C.; Chou, C.-P. Study on Mid-IR NLOCrystals CsGe(BrxCl1x)3. Opt. Mater. 2008, 31 (1), 2834.(23) Lin, Z.-G.; Tang, L.-C.; Chou, C.-P. Characterization andProperties of Infrared NLO Crystals: AGeX3 (A = Rb, Cs; X = Cl, Br).J. Cryst. Growth 2008, 310 (13), 32243229.(24) Kang, L.; Ramo, D. M.; Lin, Z.; Bristowe, P. D.; Qin, J.; Chen,C. First Principles Selection and Design of Mid-IR Nonlinear OpticalHalide Crystals. J. Mater. Chem. C 2013, 1 (44), 7363.(25) Qing-tian, G.; Chang-shui, F.; Yong-sheng, L.; Xiang-wen, W.;Qi-wei, P.; Wei, S. Growth and Properties of CsGeCl3 Single Crystal.Integr. Ferroelectr. 2001, 35 (14), 4146.(26) Lin, Z.-G.; Tang, L.-C.; Chou, C.-P. Infrared Properties ofCsGe(BrxCl1x)3, Nonlinear Optical Rhombohedral Semiconductor. J.Phys.: Condens. Matter 2007, 19, 476209.(27) Schwarz, U.; Hillebrecht, H.; Kaupp, M.; Syassen, K.; vonSchnering, H.-G.; et al. Pressure-Induced Phase Transition in CsGeBr3Studied by X-Ray Diffraction and Raman Spectroscopy. J. Solid StateChem. 1995, 118, 2027.(28) Qing-Tian, G.; Chang-Shui, F.; Wei, S.; Xiang-Wen, W.; Qi-Wei,P. New Wide-Band Nonlinear Optics CsGeCl3 Crystal. J. Cryst. Growth2001, 225 (2), 501504.(29) Tang, L. C.; Huang, J. Y.; Chang, C. S.; Lee, M. H.; Liu, L. Q.New Infrared Nonlinear Optical Crystal CsGeBr3: Synthesis, Structureand Powder Second-Harmonic Generation Properties. J. Phys.:Condens. Matter 2005, 17 (46), 72757286.(30) Veithen, M.; Gonze, X.; Ghosez, P. Nonlinear OpticalSusceptibilities, Raman Efficiencies, and Electro-Optic Tensors fromFirst-Principles Density Functional Perturbation Theory. Phys. Rev. B:Condens. Matter Mater. Phys. 2005, 71, 125107.(31) Sando, D.; Hermet, P.; Allibe, J.; Bourderionnet, J.; Fusil, S.;Carretero, C.; Jacquet, E.; Mage, J.-C.; Dolfi, D.; Barthelemy, A.; et al.Linear Electro-Optic Effect in Multiferroic BiFeO3 Thin Films. Phys.Rev. B: Condens. Matter Mater. Phys. 2014, 89, 195106.(32) Djani, H.; Hermet, P.; Ghosez, P. First-Principles Character-ization of the P21ab Ferroelectric Phase of Aurivillius Bi2WO6. J. Phys.Chem. C 2014, 118 (25), 1351413524.

The Journal of Physical Chemistry Letters Letter

DOI: 10.1021/acs.jpclett.7b03353J. Phys. Chem. Lett. 2018, 9, 10181027

1025

http://dx.doi.org/10.1021/acs.jpclett.7b03353

(33) Chen, Z.-X.; Chen, Y.; Jiang, Y.-S. DFT Study onFerroelectricity of BaTiO3. J. Phys. Chem. B 2001, 105 (24), 57665771.(34) Wang, C.-Y.; Guo, G.-Y. Nonlinear Optical Properties ofTransition-Metal Dichalcogenide MX2 (M= Mo, W; X= S, Se)Monolayers and Trilayers from First-Principles Calculations. J. Phys.Chem. C 2015, 119 (23), 1326813276.(35) Hughes, J. L.; Sipe, J. E. Calculation of Second-Order OpticalResponse in Semiconductors. Phys. Rev. B: Condens. Matter Mater.Phys. 1996, 53 (16), 10751.(36) Levine, Z. H.; Allan, D. C. Linear Optical Response in Siliconand Germanium Including Self-Energy Effects. Phys. Rev. Lett. 1989, 63(16), 1719.(37) Levine, Z. H.; Allan, D. C. Calculation of the NonlinearSusceptibility for Optical Second-Harmonic Generation in III-VSemiconductors. Phys. Rev. Lett. 1991, 66 (1), 41.(38) Levine, Z. H.; Allan, D. C. Quasiparticle Calculation of theDielectric Response of Silicon and Germanium. Phys. Rev. B: Condens.Matter Mater. Phys. 1991, 43 (5), 4187.(39) Hughes, J. L.; Wang, Y.; Sipe, J. E. Calculation of Linear andSecond-Order Optical Response in Wurtzite GaN and AlN. Phys. Rev.B: Condens. Matter Mater. Phys. 1997, 55 (20), 13630.(40) Zheng, F.; Tao, J.; Rappe, A. M. Frequency-DependentDielectric Function of Semiconductors with Application to Phys-isorption. Phys. Rev. B: Condens. Matter Mater. Phys. 2017, 95, 35203.(41) Van Troeye, B.; Gillet, Y.; Ponce, S.; Gonze, X. First-PrinciplesCharacterization of the Electronic and Optical Properties of HexagonalLiIO3. Opt. Mater. 2014, 36 (9), 14941501.(42) Song, J.-H.; Freeman, A. J.; Bera, T. K.; Chung, I.; Kanatzidis,M. G. First-Principles Prediction of an Enhanced Optical Second-Harmonic Susceptibility of Low-Dimensional Alkali-Metal Chalcoge-nides. Phys. Rev. B: Condens. Matter Mater. Phys. 2009, 79, 245203.(43) Reshak, A. H.; Atuchin, V. V.; Auluck, S.; Kityk, I. V. First andSecond Harmonic Generation of the Optical Susceptibilities for theNon-Centro-Symmetric Orthorhombic AgCd2 GaS4. J. Phys.: Condens.Matter 2008, 20 (32), 325234.(44) Kong, F.; Jiang, G. Nonlinear Optical Response of WurtziteZnO from First Principles. Phys. B 2009, 404 (16), 23402344.(45) Reshak, A. H.; Auluck, S.; Kityk, I. V. Specific Features in theBand Structure and Linear and Nonlinear Optical Susceptibilities ofLa2CaB10O19 Crystals. Phys. Rev. B: Condens. Matter Mater. Phys. 2007,75, 245120.(46) Li, Z.; Liu, Q.; Wang, Y.; Iitaka, T.; Su, H.; Tohyama, T.; Yang,Z.; Pan, S. Second-Harmonic Generation in NoncentrosymmetricPhosphates. Phys. Rev. B: Condens. Matter Mater. Phys. 2017, 96,35205.(47) Huang, L.; Lambrecht, W. R. L. Electronic Band StructureTrends of Perovskite Halides: Beyond Pb and Sn to Ge and Si. Phys.Rev. B: Condens. Matter Mater. Phys. 2016, 93, 195211.(48) Jackson, A. G.; Ohmer, M. C.; LeClair, S. R. Relationship of theSecond Order Nonlinear Optical Coefficient to Energy Gap inInorganic Non-Centrosymmetric Crystals. Infrared Phys. Technol.1997, 38 (4), 233244.(49) Yariv, A.; Yeh, P. Photonics: Optical Electronics in ModernCommunications, 6th ed.; Oxford University: New York, 2007.(50) Ghosez, P.; Michenaud, J.-P.; Gonze, X. Dynamical AtomicCharges: The Case of ABO3 Compounds. Phys. Rev. B: Condens.Matter Mater. Phys. 1998, 58 (10), 6224.(51) Marek, V. First-Principles Study of Ferroelectric Oxides:Dynamical Properties and Electron Localization Tensor. DEA Thesis;University of Liege: Leige, Belgium, 2003.(52) Peng, W.; Yin, J.; Ho, K.-T.; Ouellette, O.; De Bastiani, M.;Murali, B.; El Tall, O.; Shen, C.; Miao, X.; Pan, J.; et al. Ultralow Self-Doping in Two-Dimensional Hybrid Perovskite Single Crystals. NanoLett. 2017, 17 (8), 47594767.(53) Dang, Y.; Zhou, Y.; Liu, X.; Ju, D.; Xia, S.; Xia, H.; Tao, X.Formation of Hybrid Perovskite Tin Iodide Single Crystals by Top-Seeded Solution Growth. Angew. Chem., Int. Ed. 2016, 55 (10), 34473450.

(54) Saidaminov, M. I.; Abdelhady, A. L.; Maculan, G.; Bakr, O. M.Retrograde Solubility of Formamidinium and Methylammonium LeadHalide Perovskites Enabling Rapid Single Crystal Growth. Chem.Commun. 2015, 51 (100), 1765817661.(55) Dang, Y.; Liu, Y.; Sun, Y.; Yuan, D.; Liu, X.; Lu, W.; Liu, G.; Xia,H.; Tao, X. Bulk Crystal Growth of Hybrid Perovskite MaterialCH3NH3PbI3. CrystEngComm 2015, 17 (3), 665670.(56) Lee, L.; Baek, J.; Park, K. S.; Lee, Y.-E.; Shrestha, N. K.; Sung,M. M. Wafer-Scale Single-Crystal Perovskite Patterned Thin FilmsBased on Geometrically-Confined Lateral Crystal Growth. Nat.Commun. 2017, 8, 15882.(57) Feng, J.; Yan, X.; Zhang, Y.; Wang, X.; Wu, Y.; Su, B.; Fu, H.;Jiang, L. Liquid Knife to Fabricate Patterning Single-CrystallinePerovskite Microplates toward High-Performance Laser Arrays. Adv.Mater. 2016, 28 (19), 37323741.(58) Wang, G.; Li, D.; Cheng, H.-C.; Li, Y.; Chen, C.-Y.; Yin, A.;Zhao, Z.; Lin, Z.; Wu, H.; He, Q.; et al. Wafer-Scale Growth of LargeArrays of Perovskite Microplate Crystals for Functional Electronicsand Optoelectronics. Sci. Adv. 2015, 1, e1500613.(59) Spina, M.; Bonvin, E.; Sienkiewicz, A.; Forro, L.; Horvath, E.;et al. Controlled Growth of CH3NH3PbI3 Nanowires in Arrays ofOpen Nanofluidic Channels. Sci. Rep. 2016, 6, 19834.(60) Cho, N.; Li, F.; Turedi, B.; Sinatra, L.; Sarmah, S. P.; Parida, M.R.; Saidaminov, M. I.; Murali, B.; Burlakov, V. M.; Goriely, A.; et al.Pure Crystal Orientation and Anisotropic Charge Transport in Large-Area Hybrid Perovskite Films. Nat. Commun. 2016, 7, 13407.(61) Gonze, X.; Jollet, F.; Abreu Araujo, F.; Adams, D.; Amadon, B.;Applencourt, T.; Audouze, C.; Beuken, J.-M.; Bieder, J.; Bokhanchuk,A.; et al. Recent Developments in the ABINIT Software Package.Comput. Phys. Commun. 2016, 205, 106131.(62) Gonze, X.; Amadon, B.; Anglade, P.-M.; Beuken, J.-M.; Bottin,F.; Boulanger, P.; Bruneval, F.; Caliste, D.; Caracas, R.; Cote, M.; et al.ABINIT: First-Principles Approach to Material and NanosystemProperties. Comput. Phys. Commun. 2009, 180 (12), 25822615.(63) Gonze, X.; Rignanese, G.-M.; Verstraete, M. J.; Beuken, J.-M.;Pouillon, Y.; Caracas, R.; Jollet, F.; Torrent, M.; Zerah, G.; Mikami,M.; et al. A Brief Introduction to the ABINIT Software Package. Z.Kristallogr. - Cryst. Mater. 2005, 220, 558562.(64) Gonze, X.; Beuken, J.-M.; Caracas, R.; Detraux, F.; Fuchs, M.;Rignanese, G.-M.; Sindic, L.; Verstraete, M.; Zerah, G.; Jollet, F.; et al.First-Principles Computation of Material Properties: The ABINITSoftware Project. Comput. Mater. Sci. 2002, 25 (3), 478492.(65) Gonze, X. First-Principles Responses of Solids to AtomicDisplacements and Homogeneous Electric Fields: Implementation of aConjugate-Gradient Algorithm. Phys. Rev. B: Condens. Matter Mater.Phys. 1997, 55 (16), 10337.(66) Gonze, X.; Lee, C. Dynamical Matrices, Born Effective Charges,Dielectric Permittivity Tensors, and Interatomic Force Constants fromDensity-Functional Perturbation Theory. Phys. Rev. B: Condens. MatterMater. Phys. 1997, 55 (16), 10355.(67) Perdew, J. P.; Wang, Y. Accurate and Simple AnalyticRepresentation of the Electron-Gas Correlation Energy. Phys. Rev. B:Condens. Matter Mater. Phys. 1992, 45 (23), 1324413249.(68) Troullier, N.; Martins, J. L. Efficient Pseudopotentials for Plane-Wave Calculations. Phys. Rev. B: Condens. Matter Mater. Phys. 1991, 43(3), 1993.(69) Kurtz, S. K.; Perry, T. T. A Powder Technique for theEvaluation of Nonlinear Optical Materials. J. Appl. Phys. 1968, 39 (8),37983813.(70) Setyawan, W.; Curtarolo, S. High-Throughput Electronic BandStructure Calculations: Challenges and Tools. Comput. Mater. Sci.2010, 49 (2), 299312.(71) Giannozzi, P.; Baroni, S.; Bonini, N.; Calandra, M.; Car, R.;Cavazzoni, C.; Ceresoli, D.; Chiarotti, G. L.; Cococcioni, M.; Dabo, I.;et al. QUANTUM ESPRESSO: A Modular and Open-Source SoftwareProject for Quantum Simulations of Materials. J. Phys.: Condens. Matter2009, 21 (39), 395502.

The Journal of Physical Chemistry Letters Letter

DOI: 10.1021/acs.jpclett.7b03353J. Phys. Chem. Lett. 2018, 9, 10181027

1026

http://dx.doi.org/10.1021/acs.jpclett.7b03353

(72) Perdew, J. P.; Burke, K.; Ernzerhof, M. Generalized GradientApproximation Made Simple. Phys. Rev. Lett. 1996, 77 (18), 38653868.(73) Heyd, J.; Scuseria, G. E.; Ernzerhof, M. Hybrid FunctionalsBased on a Screened Coulomb Potential. J. Chem. Phys. 2003, 118(18), 82078215.(74) Heyd, J.; Scuseria, G. E.; Ernzerhof, M. Erratum: HybridFunctionals Based on a Screened Coulomb Potential [J. Chem. Phys.118, 8207 (2003)]. J. Chem. Phys. 2006, 124 (21), 219906.(75) Momma, K.; Izumi, F. VESTA 3 for Three-DimensionalVisualization of Crystal, Volumetric and Morphology Data. J. Appl.Crystallogr. 2011, 44 (6), 12721276.

The Journal of Physical Chemistry Letters Letter

DOI: 10.1021/acs.jpclett.7b03353J. Phys. Chem. Lett. 2018, 9, 10181027

1027

http://dx.doi.org/10.1021/acs.jpclett.7b03353